#------------------------------------------------------------------------------
#$Date: 2016-03-22 23:30:56 +0200 (Tue, 22 Mar 2016) $
#$Revision: 179064 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/26/4302606.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4302606
loop_
_publ_author_name
'Yun-Wu Li'
'Yang-Guang Li'
'Yong-Hui Wang'
'Xiao-Jia Feng'
'Ying Lu'
'En-Bo Wang'
_publ_section_title
;
A New Supramolecular Assembly Based on Triple-Dawson-Type Polyoxometalate
and 3d-4f Heterometallic Cluster
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              6452
_journal_page_last               6458
_journal_paper_doi               10.1021/ic9001362
_journal_volume                  48
_journal_year                    2009
_chemical_formula_sum            'C24 H54 Ce6 Mn10 Na20 O255 P6 W48'
_chemical_formula_weight         15283.21
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           193
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2'
_symmetry_space_group_name_H-M   'P 63/m c m'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   24.959(4)
_cell_length_b                   24.959(4)
_cell_length_c                   26.923(5)
_cell_measurement_temperature    150(2)
_cell_volume                     14525(4)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      150(2)
_diffrn_detector_area_resol_mean 0.01
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Rigaku R-AXIS RAPID IP'
_diffrn_measurement_method       Oscillation
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1399
_diffrn_reflns_av_sigmaI/netI    0.0854
_diffrn_reflns_limit_h_max       32
_diffrn_reflns_limit_h_min       -32
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       30
_diffrn_reflns_limit_l_min       -34
_diffrn_reflns_number            107511
_diffrn_reflns_theta_full        27.48
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_min         3.03
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    20.420
_exptl_absorpt_correction_T_max  0.1056
_exptl_absorpt_correction_T_min  0.0694
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'ABSCOR by T.Higashi  8 March, 1995'
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    3.495
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             13396
_exptl_crystal_size_max          0.28
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.20
_refine_diff_density_max         2.758
_refine_diff_density_min         -2.292
_refine_diff_density_rms         0.353
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.047
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     359
_refine_ls_number_reflns         5899
_refine_ls_number_restraints     54
_refine_ls_restrained_S_all      1.044
_refine_ls_R_factor_all          0.0910
_refine_ls_R_factor_gt           0.0557
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0679P)²+303.2493P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1363
_refine_ls_wR_factor_ref         0.1499
_reflns_number_gt                3946
_reflns_number_total             5899
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic9001362_si_002.cif
_cod_data_source_block           l8
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Hexagonal' changed to 'hexagonal'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_database_code               4302606
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'y, x, -z+1/2'
'x-y, -y, -z+1/2'
'-x, -x+y, -z+1/2'
'-y, -x, -z'
'-x+y, y, -z'
'x, x-y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
'-y, -x, z-1/2'
'-x+y, y, z-1/2'
'x, x-y, z-1/2'
'y, x, z'
'x-y, -y, z'
'-x, -x+y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.83392(4) 0.83392(4) 0.07108(3) 0.0190(2) Uani 1 2 d S . .
W2 W 0.67598(3) 0.75388(3) 0.06698(2) 0.01940(16) Uani 1 1 d . . .
W3 W 0.59220(3) 0.66987(3) 0.18045(2) 0.01964(16) Uani 1 1 d . . .
W4 W 0.67812(3) 0.84048(3) 0.18022(2) 0.01765(16) Uani 1 1 d . . .
W5 W 0.83288(5) 0.91481(4) 0.18392(3) 0.0179(2) Uani 0.50 1 d P . .
Mn1 Mn 0.83288(5) 0.91481(4) 0.18392(3) 0.0179(2) Uani 0.50 1 d P . .
P1 P 0.7536(2) 0.7536(2) 0.17663(19) 0.0173(11) Uani 1 2 d S . .
O1 O 0.8253(6) 0.9243(7) 0.2500 0.015(3) Uani 1 2 d S . .
O2 O 0.8845(6) 1.0000 0.1679(5) 0.022(3) Uani 1 2 d S . .
O3 O 0.8904(6) 0.8904(6) 0.1933(5) 0.022(3) Uani 1 2 d S . .
O4 O 0.8262(5) 0.8875(5) 0.1130(3) 0.017(2) Uani 1 1 d . . .
O5 O 0.8808(7) 0.8808(7) 0.0261(5) 0.023(3) Uani 1 2 d S . .
O6 O 0.6228(5) 0.7534(5) 0.1928(3) 0.018(2) Uani 1 1 d . . .
O7 O 0.6841(7) 0.8528(8) 0.2500 0.025(4) Uani 1 2 d S . .
O8 O 0.5869(7) 0.6551(7) 0.2500 0.021(3) Uani 1 2 d S . .
O9 O 0.7539(5) 0.9127(5) 0.1705(4) 0.020(2) Uani 1 1 d . . .
O10 O 0.7545(6) 0.7545(6) 0.1191(5) 0.016(3) Uani 1 2 d S . .
O11 O 0.6282(5) 0.8659(5) 0.1673(4) 0.026(3) Uani 1 1 d . . .
O12 O 0.6937(5) 0.6937(5) 0.1930(5) 0.012(3) Uani 1 2 d S . .
O13 O 0.7530(5) 0.8118(5) 0.1933(3) 0.018(2) Uani 1 1 d . . .
O14 O 0.5154(5) 0.6423(5) 0.1692(4) 0.026(3) Uani 1 1 d . . .
O15 O 0.6260(5) 0.7534(5) 0.0232(4) 0.025(3) Uani 1 1 d . . .
O16 O 0.6799(5) 0.8128(5) 0.1130(4) 0.024(3) Uani 1 1 d . . .
O17 O 0.8141(5) 0.7537(5) 0.0411(4) 0.023(2) Uani 1 1 d . . .
O18 O 0.6206(5) 0.6935(5) 0.1133(4) 0.021(2) Uani 1 1 d . . .
O19 O 0.5954(6) 0.5954(6) 0.1717(5) 0.018(3) Uani 1 2 d S . .
O20 O 0.6918(6) 0.6918(6) 0.0405(5) 0.023(3) Uani 1 2 d S . .
Ce1 Ce 0.29144(9) 0.56752(10) 0.42574(8) 0.0253(4) Uani 0.50 1 d P . .
Mn2 Mn 0.3333 0.6667 0.3363(3) 0.0219(18) Uani 0.50 3 d SP . .
Mn3 Mn 0.3333 0.6667 0.5156(3) 0.028(2) Uani 0.50 3 d SP . .
O21 O 0.3026(12) 0.5990(12) 0.2912(8) 0.033(6) Uani 0.50 1 d P . .
O22 O 0.2744(13) 0.5201(14) 0.3459(10) 0.046(8) Uani 0.50 1 d P . .
O23 O 0.3037(15) 0.5983(14) 0.5614(10) 0.041(7) Uani 0.50 1 d PU . .
O24 O 0.2599(4) 0.5198(8) 0.5000 0.038(5) Uani 1 2 d SU . .
O25 O 0.2677(12) 0.6277(12) 0.3780(9) 0.033(6) Uani 0.50 1 d PU . .
O26 O 0.2653(11) 0.6292(11) 0.4747(8) 0.028(5) Uani 0.50 1 d P . .
O27 O 0.3804(14) 0.5424(14) 0.4270(10) 0.049(7) Uani 0.50 1 d PU . .
O28 O 0.1741(11) 0.5178(11) 0.4278(9) 0.033(6) Uani 0.50 1 d PU . .
O29 O 0.2477(11) 0.4499(11) 0.4259(9) 0.033(6) Uani 0.50 1 d P . .
C1 C 0.2765(14) 0.5363(13) 0.3022(10) 0.015(6) Uani 0.50 1 d PU . .
C2 C 0.2533(15) 0.4925(15) 0.2500 0.050(8) Uani 1 2 d SU . .
C3 C 0.2713(18) 0.5364(19) 0.5454(14) 0.035(9) Uani 0.50 1 d PU . .
C4 C 0.250(2) 0.491(2) 0.5909(16) 0.044(10) Uani 0.50 1 d PU . .
Na1 Na 0.7641(9) 1.0000 0.2500 0.070(6) Uiso 1 4 d S . .
Na2 Na 0.9174(7) 0.9174(7) -0.0674(6) 0.081(5) Uiso 1 2 d S . .
Na3 Na 0.8133(8) 0.7504(7) -0.0622(5) 0.040(4) Uiso 0.50 1 d P . .
Na4 Na 0.5391(13) 0.9018(14) 0.1548(10) 0.032(6) Uiso 0.25 1 d P . .
Na5 Na 1.0000 1.0000 0.0000 0.078(11) Uiso 1 12 d S . .
Na6 Na 1.0000 1.0000 -0.1297(17) 0.058(12) Uiso 0.50 6 d SP . .
O1W O 1.0000 1.0000 0.2500 0.055(14) Uiso 1 12 d S . .
O2W O 0.6969(13) 0.6339(13) -0.0774(10) 0.041(6) Uiso 0.50 1 d P . .
O3W O 0.1008(13) 0.4698(13) 0.5015(9) 0.041(7) Uiso 0.50 1 d P . .
O4W O 0.5629(18) 0.5629(18) 0.0528(15) 0.051(11) Uiso 0.50 2 d SP . .
O5W O 0.485(2) 0.485(2) 0.131(2) 0.080(16) Uiso 0.50 2 d SP . .
O6W O 0.508(4) 0.508(4) 0.2500 0.05(2) Uiso 0.33 4 d SP . .
O7W O 0.636(5) 1.0000 0.2500 0.08(3) Uiso 0.33 4 d SP . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 W1 O4 103.0(5) . 22 ?
O5 W1 O4 103.0(5) . . ?
O4 W1 O4 92.7(6) 22 . ?
O5 W1 O17 98.3(5) . . ?
O4 W1 O17 88.3(5) 22 . ?
O4 W1 O17 157.8(5) . . ?
O5 W1 O17 98.3(5) . 22 ?
O4 W1 O17 157.8(5) 22 22 ?
O4 W1 O17 88.3(5) . 22 ?
O17 W1 O17 82.5(6) . 22 ?
O5 W1 O10 167.1(6) . . ?
O4 W1 O10 85.8(4) 22 . ?
O4 W1 O10 85.8(4) . . ?
O17 W1 O10 72.2(4) . . ?
O17 W1 O10 72.2(4) 22 . ?
O5 W1 Na2 51.5(5) . 15_655 ?
O4 W1 Na2 52.2(4) 22 15_655 ?
O4 W1 Na2 96.1(4) . 15_655 ?
O17 W1 Na2 102.0(4) . 15_655 ?
O17 W1 Na2 149.8(4) 22 15_655 ?
O10 W1 Na2 137.9(3) . 15_655 ?
O5 W1 Na2 51.5(5) . 14_565 ?
O4 W1 Na2 96.1(4) 22 14_565 ?
O4 W1 Na2 52.2(4) . 14_565 ?
O17 W1 Na2 149.8(4) . 14_565 ?
O17 W1 Na2 102.0(4) 22 14_565 ?
O10 W1 Na2 137.9(3) . 14_565 ?
Na2 W1 Na2 59.6(5) 15_655 14_565 ?
O15 W2 O16 102.1(5) . . ?
O15 W2 O17 101.9(5) . 22 ?
O16 W2 O17 89.4(5) . 22 ?
O15 W2 O18 101.9(5) . . ?
O16 W2 O18 85.5(5) . . ?
O17 W2 O18 156.2(5) 22 . ?
O15 W2 O20 100.5(5) . . ?
O16 W2 O20 157.2(5) . . ?
O17 W2 O20 87.7(6) 22 . ?
O18 W2 O20 88.0(5) . . ?
O15 W2 O10 172.2(5) . . ?
O16 W2 O10 83.6(4) . . ?
O17 W2 O10 72.6(5) 22 . ?
O18 W2 O10 83.7(4) . . ?
O20 W2 O10 74.0(4) . . ?
O14 W3 O6 103.4(5) . . ?
O14 W3 O8 98.1(6) . . ?
O6 W3 O8 89.5(5) . . ?
O14 W3 O19 99.8(5) . . ?
O6 W3 O19 156.8(5) . . ?
O8 W3 O19 88.1(6) . . ?
O14 W3 O18 97.1(5) . . ?
O6 W3 O18 86.7(4) . . ?
O8 W3 O18 164.7(6) . . ?
O19 W3 O18 89.6(6) . . ?
O14 W3 O12 172.1(5) . . ?
O6 W3 O12 84.4(4) . . ?
O8 W3 O12 82.4(5) . . ?
O19 W3 O12 72.4(4) . . ?
O18 W3 O12 82.6(4) . . ?
O11 W4 O9 100.9(5) . . ?
O11 W4 O7 98.9(6) . . ?
O9 W4 O7 91.3(6) . . ?
O11 W4 O6 102.2(5) . . ?
O9 W4 O6 156.7(5) . . ?
O7 W4 O6 87.9(6) . . ?
O11 W4 O16 95.4(5) . . ?
O9 W4 O16 91.2(4) . . ?
O7 W4 O16 164.7(6) . . ?
O6 W4 O16 83.9(4) . . ?
O11 W4 O13 175.1(5) . . ?
O9 W4 O13 74.8(4) . . ?
O7 W4 O13 83.7(5) . . ?
O6 W4 O13 82.0(4) . . ?
O16 W4 O13 82.4(4) . . ?
O1 W5 O3 93.3(7) . . ?
O1 W5 O2 97.6(6) . . ?
O3 W5 O2 101.3(7) . . ?
O1 W5 O9 90.9(5) . . ?
O3 W5 O9 161.8(6) . . ?
O2 W5 O9 95.6(5) . . ?
O1 W5 O4 168.4(5) . . ?
O3 W5 O4 88.0(5) . . ?
O2 W5 O4 93.4(5) . . ?
O9 W5 O4 84.5(4) . . ?
O1 W5 O13 87.2(5) . . ?
O3 W5 O13 89.9(6) . . ?
O2 W5 O13 167.4(5) . . ?
O9 W5 O13 72.6(4) . . ?
O4 W5 O13 81.4(4) . . ?
O13 P1 O13 112.7(9) 22 . ?
O13 P1 O10 106.7(5) 22 . ?
O13 P1 O10 106.7(5) . . ?
O13 P1 O12 111.6(5) 22 . ?
O13 P1 O12 111.6(5) . . ?
O10 P1 O12 107.2(8) . . ?
Mn1 O1 W5 0.00(7) 16_556 16_556 ?
Mn1 O1 W5 156.5(10) 16_556 . ?
W5 O1 W5 156.5(10) 16_556 . ?
Mn1 O1 Na1 101.7(5) 16_556 . ?
W5 O1 Na1 101.7(5) 16_556 . ?
W5 O1 Na1 101.7(5) . . ?
Mn1 O2 W5 0.00(8) 23_675 23_675 ?
Mn1 O2 W5 150.4(8) 23_675 . ?
W5 O2 W5 150.4(8) 23_675 . ?
Mn1 O2 Na2 104.5(4) 23_675 14_565 ?
W5 O2 Na2 104.5(4) 23_675 14_565 ?
W5 O2 Na2 104.5(4) . 14_565 ?
Mn1 O3 W5 0.00(6) 22 22 ?
Mn1 O3 W5 149.4(9) 22 . ?
W5 O3 W5 149.4(9) 22 . ?
W1 O4 W5 144.3(6) . . ?
W1 O4 Na2 97.5(5) . 14_565 ?
W5 O4 Na2 100.7(5) . 14_565 ?
W1 O5 Na2 156.0(9) . . ?
W1 O5 Na2 101.1(6) . 15_655 ?
Na2 O5 Na2 97.6(7) . 15_655 ?
W1 O5 Na2 101.1(6) . 14_565 ?
Na2 O5 Na2 97.6(7) . 14_565 ?
Na2 O5 Na2 77.1(8) 15_655 14_565 ?
W3 O6 W4 153.1(6) . . ?
W4 O7 W4 163.9(10) 16_556 . ?
W3 O8 W3 160.4(9) 16_556 . ?
W4 O9 W5 121.0(5) . . ?
W4 O9 Na1 106.3(5) . . ?
W5 O9 Na1 97.4(6) . . ?
W4 O9 Na3 102.4(5) . 14_565 ?
W5 O9 Na3 107.7(5) . 14_565 ?
Na1 O9 Na3 123.6(5) . 14_565 ?
P1 O10 W1 123.8(8) . . ?
P1 O10 W2 125.3(4) . 22 ?
W1 O10 W2 91.5(4) . 22 ?
P1 O10 W2 125.3(4) . . ?
W1 O10 W2 91.5(4) . . ?
W2 O10 W2 89.0(5) 22 . ?
W4 O11 Na4 174.2(8) . . ?
P1 O12 W3 127.3(4) . 22 ?
P1 O12 W3 127.3(4) . . ?
W3 O12 W3 92.7(5) 22 . ?
P1 O13 W4 129.6(6) . . ?
P1 O13 W5 127.0(6) . . ?
W4 O13 W5 91.2(4) . . ?
W2 O16 W4 152.4(7) . . ?
W2 O17 W1 123.7(6) 22 . ?
W2 O17 Na3 110.3(6) 22 . ?
W1 O17 Na3 115.7(6) . . ?
W2 O18 W3 149.9(6) . . ?
W3 O19 W3 122.5(8) 22 . ?
W2 O20 W2 122.9(7) 22 . ?
O23 Ce1 C3 96(3) 11_556 11_556 ?
O23 Ce1 C4 145(3) 11_556 11_556 ?
C3 Ce1 C4 63(3) 11_556 11_556 ?
O23 Ce1 O24 88(2) 11_556 . ?
C3 Ce1 O24 17(2) 11_556 . ?
C4 Ce1 O24 77.1(15) 11_556 . ?
O23 Ce1 O25 63(2) 11_556 . ?
C3 Ce1 O25 129(2) 11_556 . ?
C4 Ce1 O25 106.9(16) 11_556 . ?
O24 Ce1 O25 135.5(6) . . ?
O23 Ce1 O26 54(2) 11_556 2_665 ?
C3 Ce1 O26 97(2) 11_556 2_665 ?
C4 Ce1 O26 148.8(15) 11_556 2_665 ?
O24 Ce1 O26 80.0(6) . 2_665 ?
O25 Ce1 O26 104.3(8) . 2_665 ?
O23 Ce1 O25 82(2) 11_556 2_665 ?
C3 Ce1 O25 163(2) 11_556 2_665 ?
C4 Ce1 O25 126.1(16) 11_556 2_665 ?
O24 Ce1 O25 147.4(7) . 2_665 ?
O25 Ce1 O25 65.3(13) . 2_665 ?
O26 Ce1 O25 69.1(8) 2_665 2_665 ?
O23 Ce1 O26 21(2) 11_556 . ?
C3 Ce1 O26 78(2) 11_556 . ?
C4 Ce1 O26 124.8(15) 11_556 . ?
O24 Ce1 O26 73.2(7) . . ?
O25 Ce1 O26 68.6(8) . . ?
O26 Ce1 O26 66.8(12) 2_665 . ?
O25 Ce1 O26 102.7(9) 2_665 . ?
O23 Ce1 O22 140(2) 11_556 . ?
C3 Ce1 O22 114(2) 11_556 . ?
C4 Ce1 O22 51.3(16) 11_556 . ?
O24 Ce1 O22 127.4(9) . . ?
O25 Ce1 O22 77.1(10) . . ?
O26 Ce1 O22 139.9(9) 2_665 . ?
O25 Ce1 O22 75.9(10) 2_665 . ?
O26 Ce1 O22 142.2(9) . . ?
O23 Ce1 O28 90(2) 11_556 . ?
C3 Ce1 O28 59(2) 11_556 . ?
C4 Ce1 O28 55.9(15) 11_556 . ?
O24 Ce1 O28 73.2(6) . . ?
O25 Ce1 O28 73.6(9) . . ?
O26 Ce1 O28 135.1(8) 2_665 . ?
O25 Ce1 O28 137.3(8) 2_665 . ?
O26 Ce1 O28 71.3(8) . . ?
O22 Ce1 O28 84.4(9) . . ?
O23 Ce1 O29 150(2) 11_556 . ?
C3 Ce1 O29 54(2) 11_556 . ?
C4 Ce1 O29 24.3(15) 11_556 . ?
O24 Ce1 O29 63.8(7) . . ?
O25 Ce1 O29 130.9(9) . . ?
O26 Ce1 O29 124.7(8) 2_665 . ?
O25 Ce1 O29 126.9(8) 2_665 . ?
O26 Ce1 O29 130.4(8) . . ?
O22 Ce1 O29 64.3(10) . . ?
O28 Ce1 O29 73.5(8) . . ?
O23 Ce1 O27 122(2) 11_556 . ?
C3 Ce1 O27 96(2) 11_556 . ?
C4 Ce1 O27 89.0(16) 11_556 . ?
O24 Ce1 O27 88.6(6) . . ?
O25 Ce1 O27 135.0(9) . . ?
O26 Ce1 O27 69.3(9) 2_665 . ?
O25 Ce1 O27 71.3(9) 2_665 . ?
O26 Ce1 O27 134.6(9) . . ?
O22 Ce1 O27 81.6(9) . . ?
O28 Ce1 O27 142.9(9) . . ?
O29 Ce1 O27 69.5(9) . . ?
O25 Mn2 O25 85.8(12) 3_565 . ?
O25 Mn2 O25 85.8(12) 3_565 2_665 ?
O25 Mn2 O25 85.8(12) . 2_665 ?
O25 Mn2 O21 93.6(11) 3_565 3_565 ?
O25 Mn2 O21 96.9(11) . 3_565 ?
O25 Mn2 O21 177.2(11) 2_665 3_565 ?
O25 Mn2 O21 177.2(11) 3_565 . ?
O25 Mn2 O21 93.6(11) . . ?
O25 Mn2 O21 96.9(11) 2_665 . ?
O21 Mn2 O21 83.7(11) 3_565 . ?
O25 Mn2 O21 96.9(11) 3_565 2_665 ?
O25 Mn2 O21 177.2(11) . 2_665 ?
O25 Mn2 O21 93.6(11) 2_665 2_665 ?
O21 Mn2 O21 83.7(11) 3_565 2_665 ?
O21 Mn2 O21 83.7(11) . 2_665 ?
O25 Mn2 Ce1 43.0(8) 3_565 3_565 ?
O25 Mn2 Ce1 44.4(8) . 3_565 ?
O25 Mn2 Ce1 93.6(9) 2_665 3_565 ?
O21 Mn2 Ce1 87.9(7) 3_565 3_565 ?
O21 Mn2 Ce1 135.7(8) . 3_565 ?
O21 Mn2 Ce1 138.4(7) 2_665 3_565 ?
O25 Mn2 Ce1 44.4(8) 3_565 2_665 ?
O25 Mn2 Ce1 93.6(9) . 2_665 ?
O25 Mn2 Ce1 43.0(8) 2_665 2_665 ?
O21 Mn2 Ce1 135.7(8) 3_565 2_665 ?
O21 Mn2 Ce1 138.4(7) . 2_665 ?
O21 Mn2 Ce1 87.9(7) 2_665 2_665 ?
Ce1 Mn2 Ce1 70.48(17) 3_565 2_665 ?
O25 Mn2 Ce1 93.6(9) 3_565 . ?
O25 Mn2 Ce1 43.0(8) . . ?
O25 Mn2 Ce1 44.4(8) 2_665 . ?
O21 Mn2 Ce1 138.4(7) 3_565 . ?
O21 Mn2 Ce1 87.9(7) . . ?
O21 Mn2 Ce1 135.7(8) 2_665 . ?
Ce1 Mn2 Ce1 70.48(17) 3_565 . ?
Ce1 Mn2 Ce1 70.48(17) 2_665 . ?
Mn3 Mn3 O26 100.1(10) 10_666 12_566 ?
Mn3 Mn3 O26 100.1(10) 10_666 10_666 ?
O26 Mn3 O26 117.0(6) 12_566 10_666 ?
Mn3 Mn3 O26 100.1(9) 10_666 11_556 ?
O26 Mn3 O26 117.0(6) 12_566 11_556 ?
O26 Mn3 O26 117.0(6) 10_666 11_556 ?
Mn3 Mn3 O26 53.3(7) 10_666 . ?
O26 Mn3 O26 47.2(15) 12_566 . ?
O26 Mn3 O26 125.2(14) 10_666 . ?
O26 Mn3 O26 114.6(16) 11_556 . ?
Mn3 Mn3 O26 53.3(7) 10_666 3_565 ?
O26 Mn3 O26 114.6(16) 12_566 3_565 ?
O26 Mn3 O26 47.2(15) 10_666 3_565 ?
O26 Mn3 O26 125.2(14) 11_556 3_565 ?
O26 Mn3 O26 87.9(11) . 3_565 ?
Mn3 Mn3 O26 53.3(7) 10_666 2_665 ?
O26 Mn3 O26 125.2(14) 12_566 2_665 ?
O26 Mn3 O26 114.6(16) 10_666 2_665 ?
O26 Mn3 O26 47.2(15) 11_556 2_665 ?
O26 Mn3 O26 87.9(11) . 2_665 ?
O26 Mn3 O26 87.9(11) 3_565 2_665 ?
Mn3 Mn3 O23 129.8(8) 10_666 3_565 ?
O26 Mn3 O23 54.9(12) 12_566 3_565 ?
O26 Mn3 O23 66.5(13) 10_666 3_565 ?
O26 Mn3 O23 129.6(13) 11_556 3_565 ?
O26 Mn3 O23 93.8(11) . 3_565 ?
O26 Mn3 O23 94.8(12) 3_565 3_565 ?
O26 Mn3 O23 176.8(12) 2_665 3_565 ?
Mn3 Mn3 O23 129.8(9) 10_666 2_665 ?
O26 Mn3 O23 129.6(13) 12_566 2_665 ?
O26 Mn3 O23 54.9(12) 10_666 2_665 ?
O26 Mn3 O23 66.5(13) 11_556 2_665 ?
O26 Mn3 O23 176.8(11) . 2_665 ?
O26 Mn3 O23 93.8(11) 3_565 2_665 ?
O26 Mn3 O23 94.8(12) 2_665 2_665 ?
O23 Mn3 O23 83.4(13) 3_565 2_665 ?
Mn3 Mn3 O23 129.8(8) 10_666 . ?
O26 Mn3 O23 66.5(13) 12_566 . ?
O26 Mn3 O23 129.6(13) 10_666 . ?
O26 Mn3 O23 54.9(12) 11_556 . ?
O26 Mn3 O23 94.8(12) . . ?
O26 Mn3 O23 176.8(12) 3_565 . ?
O26 Mn3 O23 93.8(11) 2_665 . ?
O23 Mn3 O23 83.4(13) 3_565 . ?
O23 Mn3 O23 83.4(13) 2_665 . ?
Mn3 Mn3 Ce1 126.30(15) 10_666 12_566 ?
O26 Mn3 Ce1 61.4(8) 12_566 12_566 ?
O26 Mn3 Ce1 58.6(10) 10_666 12_566 ?
O26 Mn3 Ce1 133.6(10) 11_556 12_566 ?
O26 Mn3 Ce1 96.7(7) . 12_566 ?
O26 Mn3 Ce1 87.3(8) 3_565 12_566 ?
O26 Mn3 Ce1 173.2(7) 2_665 12_566 ?
O23 Mn3 Ce1 8.3(9) 3_565 12_566 ?
O23 Mn3 Ce1 80.7(10) 2_665 12_566 ?
O23 Mn3 Ce1 90.9(9) . 12_566 ?
Mn3 Mn3 Ce1 126.30(15) 10_666 10_666 ?
O26 Mn3 Ce1 133.6(10) 12_566 10_666 ?
O26 Mn3 Ce1 61.4(8) 10_666 10_666 ?
O26 Mn3 Ce1 58.6(10) 11_556 10_666 ?
O26 Mn3 Ce1 173.2(7) . 10_666 ?
O26 Mn3 Ce1 96.7(7) 3_565 10_666 ?
O26 Mn3 Ce1 87.3(8) 2_665 10_666 ?
O23 Mn3 Ce1 90.9(9) 3_565 10_666 ?
O23 Mn3 Ce1 8.3(9) 2_665 10_666 ?
O23 Mn3 Ce1 80.7(10) . 10_666 ?
Ce1 Mn3 Ce1 88.5(2) 12_566 10_666 ?
C1 O21 Mn2 128.0(18) . . ?
C1 O22 C4 158(3) . 11_556 ?
C1 O22 Ce1 137(2) . . ?
C4 O22 Ce1 46.6(14) 11_556 . ?
Ce1 O23 C3 49(2) 11_556 . ?
Ce1 O23 O26 149(3) 11_556 11_556 ?
C3 O23 O26 103(2) . 11_556 ?
Ce1 O23 Mn3 152(3) 11_556 . ?
C3 O23 Mn3 122(2) . . ?
O26 O23 Mn3 48.8(12) 11_556 . ?
C3 O24 C3 147(4) . 11_556 ?
C3 O24 Ce1 13.8(18) . 11_556 ?
C3 O24 Ce1 136(2) 11_556 11_556 ?
C3 O24 Ce1 136(2) . . ?
C3 O24 Ce1 13.8(18) 11_556 . ?
Ce1 O24 Ce1 125.7(8) 11_556 . ?
Mn2 O25 Ce1 103.9(11) . . ?
Mn2 O25 Ce1 102.3(12) . 3_565 ?
Ce1 O25 Ce1 108.8(10) . 3_565 ?
O26 O26 Mn3 79.6(9) 12_566 10_666 ?
O26 O26 O23 133(3) 12_566 11_556 ?
Mn3 O26 O23 76.3(15) 10_666 11_556 ?
O26 O26 Mn3 53.2(7) 12_566 . ?
Mn3 O26 Mn3 26.7(7) 10_666 . ?
O23 O26 Mn3 94.6(16) 11_556 . ?
O26 O26 Ce1 118(2) 12_566 3_565 ?
Mn3 O26 Ce1 87.4(11) 10_666 3_565 ?
O23 O26 Ce1 100.4(15) 11_556 3_565 ?
Mn3 O26 Ce1 103.1(11) . 3_565 ?
O26 O26 Ce1 131(2) 12_566 . ?
Mn3 O26 Ce1 84.7(10) 10_666 . ?
O23 O26 Ce1 10.3(11) 11_556 . ?
Mn3 O26 Ce1 100.4(10) . . ?
Ce1 O26 Ce1 107.0(9) 3_565 . ?
Ce1 O27 Na4 108.3(12) . 18_566 ?
C4 O29 Ce1 36(2) 11_556 . ?
O22 C1 O21 119(3) . . ?
O22 C1 C2 129(3) . . ?
O21 C1 C2 111(2) . . ?
C1 C2 C1 112(3) . 16_556 ?
Ce1 C3 O24 150(4) 11_556 . ?
Ce1 C3 O23 34.8(17) 11_556 . ?
O24 C3 O23 124(3) . . ?
Ce1 C3 C4 81(3) 11_556 . ?
O24 C3 C4 125(4) . . ?
O23 C3 C4 111(3) . . ?
O29 C4 C3 98(3) 11_556 . ?
O29 C4 Ce1 119(3) 11_556 11_556 ?
C3 C4 Ce1 36.8(17) . 11_556 ?
O29 C4 O22 116(3) 11_556 11_556 ?
C3 C4 O22 119(3) . 11_556 ?
Ce1 C4 O22 82(2) 11_556 11_556 ?
O1 Na1 O1 67.0(7) 8_675 . ?
O1 Na1 O9 54.2(3) 8_675 8_675 ?
O1 Na1 O9 96.7(6) . 8_675 ?
O1 Na1 O9 96.7(6) 8_675 16_556 ?
O1 Na1 O9 54.2(3) . 16_556 ?
O9 Na1 O9 78.8(4) 8_675 16_556 ?
O1 Na1 O9 96.7(6) 8_675 . ?
O1 Na1 O9 54.2(3) . . ?
O9 Na1 O9 147.4(9) 8_675 . ?
O9 Na1 O9 92.1(5) 16_556 . ?
O1 Na1 O9 54.2(3) 8_675 23_675 ?
O1 Na1 O9 96.7(6) . 23_675 ?
O9 Na1 O9 92.1(5) 8_675 23_675 ?
O9 Na1 O9 147.4(9) 16_556 23_675 ?
O9 Na1 O9 78.8(4) . 23_675 ?
Na6 Na2 O5 149.1(11) . . ?
Na6 Na2 Na5 80.5(9) . . ?
O5 Na2 Na5 68.6(5) . . ?
Na6 Na2 O2 67.7(9) . 15_655 ?
O5 Na2 O2 143.2(8) . 15_655 ?
Na5 Na2 O2 148.2(7) . 15_655 ?
Na6 Na2 O4 88.0(6) . 15_655 ?
O5 Na2 O4 107.4(5) . 15_655 ?
Na5 Na2 O4 120.8(4) . 15_655 ?
O2 Na2 O4 60.0(3) 15_655 15_655 ?
Na6 Na2 O4 88.0(6) . 12_565 ?
O5 Na2 O4 107.4(5) . 12_565 ?
Na5 Na2 O4 120.8(4) . 12_565 ?
O2 Na2 O4 60.0(3) 15_655 12_565 ?
O4 Na2 O4 116.4(7) 15_655 12_565 ?
Na6 Na2 O5 95.1(5) . 15_655 ?
O5 Na2 O5 72.8(4) . 15_655 ?
Na5 Na2 O5 66.0(4) . 15_655 ?
O2 Na2 O5 115.4(4) 15_655 15_655 ?
O4 Na2 O5 57.5(4) 15_655 15_655 ?
O4 Na2 O5 172.9(7) 12_565 15_655 ?
Na6 Na2 O5 95.1(5) . 14_565 ?
O5 Na2 O5 72.8(4) . 14_565 ?
Na5 Na2 O5 66.0(4) . 14_565 ?
O2 Na2 O5 115.4(4) 15_655 14_565 ?
O4 Na2 O5 172.9(7) 15_655 14_565 ?
O4 Na2 O5 57.5(4) 12_565 14_565 ?
O5 Na2 O5 128.2(8) 15_655 14_565 ?
Na6 Na2 Na2 47.8(6) . 2_765 ?
O5 Na2 Na2 107.2(4) . 2_765 ?
Na5 Na2 Na2 49.4(3) . 2_765 ?
O2 Na2 Na2 104.5(4) 15_655 2_765 ?
O4 Na2 Na2 80.7(4) 15_655 2_765 ?
O4 Na2 Na2 133.6(4) 12_565 2_765 ?
O5 Na2 Na2 51.4(4) 15_655 2_765 ?
O5 Na2 Na2 106.0(4) 14_565 2_765 ?
Na6 Na2 Na2 47.8(6) . 3_675 ?
O5 Na2 Na2 107.2(4) . 3_675 ?
Na5 Na2 Na2 49.4(3) . 3_675 ?
O2 Na2 Na2 104.5(4) 15_655 3_675 ?
O4 Na2 Na2 133.6(4) 15_655 3_675 ?
O4 Na2 Na2 80.7(4) 12_565 3_675 ?
O5 Na2 Na2 106.0(4) 15_655 3_675 ?
O5 Na2 Na2 51.4(4) 14_565 3_675 ?
Na2 Na2 Na2 60.000(1) 2_765 3_675 ?
Na6 Na2 W1 89.1(3) . 15_655 ?
O5 Na2 W1 91.4(3) . 15_655 ?
Na5 Na2 W1 91.2(3) . 15_655 ?
O2 Na2 W1 88.4(3) 15_655 15_655 ?
O4 Na2 W1 30.4(2) 15_655 15_655 ?
O4 Na2 W1 146.8(6) 12_565 15_655 ?
O5 Na2 W1 27.4(3) 15_655 15_655 ?
O5 Na2 W1 155.6(6) 14_565 15_655 ?
Na2 Na2 W1 60.2(3) 2_765 15_655 ?
Na2 Na2 W1 120.2(3) 3_675 15_655 ?
Na6 Na2 W1 89.1(3) . 14_565 ?
O5 Na2 W1 91.4(3) . 14_565 ?
Na5 Na2 W1 91.2(3) . 14_565 ?
O2 Na2 W1 88.4(3) 15_655 14_565 ?
O4 Na2 W1 146.8(6) 15_655 14_565 ?
O4 Na2 W1 30.4(2) 12_565 14_565 ?
O5 Na2 W1 155.6(6) 15_655 14_565 ?
O5 Na2 W1 27.4(3) 14_565 14_565 ?
Na2 Na2 W1 120.2(3) 2_765 14_565 ?
Na2 Na2 W1 60.2(3) 3_675 14_565 ?
W1 Na2 W1 176.8(5) 15_655 14_565 ?
Na3 Na3 O17 88.8(4) 22 . ?
Na3 Na3 O2W 90.0(6) 22 . ?
O17 Na3 O2W 99.1(7) . . ?
Na3 Na3 O9 100.1(4) 22 15_655 ?
O17 Na3 O9 167.5(7) . 15_655 ?
O2W Na3 O9 89.7(7) . 15_655 ?
Na3 Na3 Na2 68.1(3) 22 . ?
O17 Na3 Na2 90.7(5) . . ?
O2W Na3 Na2 155.9(8) . . ?
O9 Na3 Na2 84.7(5) 15_655 . ?
O11 Na4 O5W 146.8(15) . 2_665 ?
O11 Na4 O27 111.6(11) . 17_666 ?
O5W Na4 O27 85.0(13) 2_665 17_666 ?
O11 Na4 O2W 62.1(8) . 14_565 ?
O5W Na4 O2W 93.8(15) 2_665 14_565 ?
O27 Na4 O2W 82.1(10) 17_666 14_565 ?
Na2 Na5 Na2 180.000(1) 13_775 . ?
Na2 Na5 Na2 81.1(5) 13_775 15_655 ?
Na2 Na5 Na2 98.9(5) . 15_655 ?
Na2 Na5 Na2 81.1(5) 13_775 14_565 ?
Na2 Na5 Na2 98.9(5) . 14_565 ?
Na2 Na5 Na2 81.1(5) 15_655 14_565 ?
Na2 Na5 Na2 98.9(5) 13_775 2_765 ?
Na2 Na5 Na2 81.1(5) . 2_765 ?
Na2 Na5 Na2 98.9(5) 15_655 2_765 ?
Na2 Na5 Na2 180.000(1) 14_565 2_765 ?
Na2 Na5 Na2 98.9(5) 13_775 3_675 ?
Na2 Na5 Na2 81.1(5) . 3_675 ?
Na2 Na5 Na2 180.0(7) 15_655 3_675 ?
Na2 Na5 Na2 98.9(5) 14_565 3_675 ?
Na2 Na5 Na2 81.1(5) 2_765 3_675 ?
Na2 Na5 Na6 48.7(3) 13_775 13_775 ?
Na2 Na5 Na6 131.3(3) . 13_775 ?
Na2 Na5 Na6 48.7(3) 15_655 13_775 ?
Na2 Na5 Na6 48.7(3) 14_565 13_775 ?
Na2 Na5 Na6 131.3(3) 2_765 13_775 ?
Na2 Na5 Na6 131.3(3) 3_675 13_775 ?
Na2 Na5 Na6 131.3(3) 13_775 . ?
Na2 Na5 Na6 48.7(3) . . ?
Na2 Na5 Na6 131.3(3) 15_655 . ?
Na2 Na5 Na6 131.3(3) 14_565 . ?
Na2 Na5 Na6 48.7(3) 2_765 . ?
Na2 Na5 Na6 48.7(3) 3_675 . ?
Na6 Na5 Na6 180.000(2) 13_775 . ?
Na2 Na6 Na2 84.4(12) 2_765 3_675 ?
Na2 Na6 Na2 84.4(12) 2_765 . ?
Na2 Na6 Na2 84.4(12) 3_675 . ?
Na2 Na6 Na5 50.8(8) 2_765 . ?
Na2 Na6 Na5 50.8(8) 3_675 . ?
Na2 Na6 Na5 50.8(8) . . ?
Na3 O2W Na4 138.4(11) . 15_655 ?
Na4 O5W Na4 96(2) 24_655 3_565 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O5 1.684(16) . ?
W1 O4 1.832(10) 22 ?
W1 O4 1.832(10) . ?
W1 O17 1.977(11) . ?
W1 O17 1.977(11) 22 ?
W1 O10 2.367(14) . ?
W1 Na2 3.5913(10) 15_655 ?
W1 Na2 3.5913(10) 14_565 ?
W2 O15 1.713(11) . ?
W2 O16 1.888(11) . ?
W2 O17 1.896(11) 22 ?
W2 O18 1.913(11) . ?
W2 O20 1.917(7) . ?
W2 O10 2.403(10) . ?
W3 O14 1.710(10) . ?
W3 O6 1.857(11) . ?
W3 O8 1.900(3) . ?
W3 O19 1.915(7) . ?
W3 O18 1.923(10) . ?
W3 O12 2.319(9) . ?
W4 O11 1.691(11) . ?
W4 O9 1.867(10) . ?
W4 O7 1.897(2) . ?
W4 O6 1.935(10) . ?
W4 O16 1.946(10) . ?
W4 O13 2.337(11) . ?
W5 O1 1.817(3) . ?
W5 O3 1.836(4) . ?
W5 O2 1.905(4) . ?
W5 O9 1.979(10) . ?
W5 O4 2.007(9) . ?
W5 O13 2.350(11) . ?
P1 O13 1.528(11) 22 ?
P1 O13 1.528(11) . ?
P1 O10 1.550(14) . ?
P1 O12 1.560(14) . ?
O1 Mn1 1.817(3) 16_556 ?
O1 W5 1.817(3) 16_556 ?
O1 Na1 2.96(2) . ?
O2 Mn1 1.905(4) 23_675 ?
O2 W5 1.905(4) 23_675 ?
O2 Na2 2.83(2) 14_565 ?
O3 Mn1 1.836(4) 22 ?
O3 W5 1.836(4) 22 ?
O4 Na2 2.860(13) 14_565 ?
O5 Na2 2.68(2) . ?
O5 Na2 2.864(14) 15_655 ?
O5 Na2 2.864(14) 14_565 ?
O7 W4 1.897(2) 16_556 ?
O8 W3 1.900(3) 16_556 ?
O9 Na1 2.973(12) . ?
O9 Na3 2.987(17) 14_565 ?
O10 W2 2.403(10) 22 ?
O11 Na4 2.81(3) . ?
O12 W3 2.319(9) 22 ?
O17 W2 1.896(11) 22 ?
O17 Na3 2.783(18) . ?
O19 W3 1.915(7) 22 ?
O20 W2 1.917(7) 22 ?
Ce1 O23 0.81(3) 11_556 ?
Ce1 C3 1.06(4) 11_556 ?
Ce1 C4 1.75(4) 11_556 ?
Ce1 O24 2.258(8) . ?
Ce1 O25 2.27(3) . ?
Ce1 O26 2.28(2) 2_665 ?
Ce1 O25 2.31(2) 2_665 ?
Ce1 O26 2.35(2) . ?
Ce1 O22 2.39(3) . ?
Ce1 O28 2.55(2) . ?
Ce1 O29 2.57(2) . ?
Ce1 O27 2.59(3) . ?
Mn2 O25 1.82(2) 3_565 ?
Mn2 O25 1.82(2) . ?
Mn2 O25 1.82(2) 2_665 ?
Mn2 O21 1.90(2) 3_565 ?
Mn2 O21 1.90(2) . ?
Mn2 O21 1.90(2) 2_665 ?
Mn2 Ce1 3.229(7) 3_565 ?
Mn2 Ce1 3.229(7) 2_665 ?
Mn3 Mn3 0.838(17) 10_666 ?
Mn3 O26 1.50(2) 12_566 ?
Mn3 O26 1.50(2) 10_666 ?
Mn3 O26 1.50(2) 11_556 ?
Mn3 O26 1.84(2) . ?
Mn3 O26 1.84(2) 3_565 ?
Mn3 O26 1.84(2) 2_665 ?
Mn3 O23 1.93(3) 3_565 ?
Mn3 O23 1.93(3) 2_665 ?
Mn3 O23 1.93(3) . ?
Mn3 Ce1 2.670(5) 12_566 ?
Mn3 Ce1 2.670(5) 10_666 ?
O21 C1 1.39(4) . ?
O22 C1 1.24(4) . ?
O22 C4 1.88(5) 11_556 ?
O23 Ce1 0.81(3) 11_556 ?
O23 C3 1.41(5) . ?
O23 O26 1.62(4) 11_556 ?
O24 C3 1.27(4) . ?
O24 C3 1.27(4) 11_556 ?
O24 Ce1 2.258(8) 11_556 ?
O25 Ce1 2.31(2) 3_565 ?
O26 O26 1.37(4) 12_566 ?
O26 Mn3 1.50(2) 10_666 ?
O26 O23 1.62(4) 11_556 ?
O26 Ce1 2.28(2) 3_565 ?
O27 Na4 2.88(4) 18_566 ?
O29 C4 1.21(5) 11_556 ?
C1 C2 1.69(3) . ?
C2 C1 1.69(3) 16_556 ?
C3 Ce1 1.06(4) 11_556 ?
C3 C4 1.58(6) . ?
C4 O29 1.21(5) 11_556 ?
C4 Ce1 1.75(4) 11_556 ?
C4 O22 1.88(5) 11_556 ?
Na1 O1 2.96(2) 8_675 ?
Na1 O9 2.973(12) 8_675 ?
Na1 O9 2.973(12) 16_556 ?
Na1 O9 2.973(12) 23_675 ?
Na2 Na6 2.66(3) . ?
Na2 Na5 2.746(17) . ?
Na2 O2 2.83(2) 15_655 ?
Na2 O4 2.860(13) 15_655 ?
Na2 O4 2.860(13) 12_565 ?
Na2 O5 2.864(14) 15_655 ?
Na2 O5 2.864(14) 14_565 ?
Na2 Na2 3.57(3) 2_765 ?
Na2 Na2 3.57(3) 3_675 ?
Na2 W1 3.5913(10) 15_655 ?
Na2 W1 3.5913(10) 14_565 ?
Na3 Na3 2.72(3) 22 ?
Na3 O2W 2.94(3) . ?
Na3 O9 2.987(17) 15_655 ?
Na4 O5W 2.86(5) 2_665 ?
Na4 O27 2.88(4) 17_666 ?
Na4 O2W 2.94(4) 14_565 ?
Na5 Na2 2.746(17) 13_775 ?
Na5 Na2 2.746(17) 15_655 ?
Na5 Na2 2.746(17) 14_565 ?
Na5 Na2 2.746(17) 2_765 ?
Na5 Na2 2.746(17) 3_675 ?
Na5 Na6 3.49(5) 13_775 ?
Na5 Na6 3.49(5) . ?
Na6 Na2 2.66(3) 2_765 ?
Na6 Na2 2.66(3) 3_675 ?
O2W Na4 2.94(4) 15_655 ?
O5W Na4 2.86(5) 24_655 ?
O5W Na4 2.86(5) 3_565 ?
